Theories and Methods of First Order Ferroelectric Phase Transitions


 Hortense Waters
 3 years ago
 Views:
Transcription
1 16 Theories and Methods of First Order Ferroelectric Phase Transitions C L Wang Shandong University P R China 1. Introduction Most ferroelectrics in practical applications are of first order phase transition, such as barium titanate, lead zirconium titanate, etc. However, theoretical investigation of first order phase transition is much more complicated than that of second order phase transitions. Therefore in the chapter, theoretical treatments of ferroelectric phase transition of first order are summarized. In the next section, results from thermodynamic theory are discussed. This kind of theory is often called Landau theory, LandauDevonshire theory or Landau Devoshire Ginzburg theory in literatures. Basic concepts and definitions such as characteristic temperatures, thermal hysteresis and field induced phase transition are presented. In the third section, effective field approach for first order phase transition is formulised. Even though this approach is a very simple statistic physics method, it supplies a very helpful approach to understand many physical phenomena of first order phase transitions. In the fourth section, results from Ising model in a transverse field under mean field approximation are discussed. Then the equivalence of the model with effective field approach is demonstrated. Also application of Monte Carlo simulation on Ising model with fourspin couplings is included. In the last part, understanding of physical property of relaxor ferroelectrics from point view of first order phase transition is addressed.. Thermodynamic theory of ferroelectrics In this section, thermodynamic theory of first order ferroelectric phase transition is formalized. Free energy is analyzed at first. Then definition of characteristic temperatures is discussed. Afterwards temperature dependence of polarization and hysteresis loops are shown for static situation. At last dynamic behavior of polarization under external electric field is presented. Formalism of thermodynamic description, or Landau theory for ferroelectrics can be found in many classical books (Blinc & Zeks,1974; Lines & Glass, 1977), or from website like wikipedia ( Based on Landau theory, the free energy of a ferroelectric material, in the absence of an electric field and applied stress may be written as a Taylor expansion in terms of the order parameter, polarization (P). If a sixth order expansion is used (i.e. eighth order and higher terms truncated), the free energy is given by:
2 76 Ferroelectrics Δ G = α0 TTPPP α 11 PPP α 1 PPPPPP α 111 ( PPP ) 11 ( ) ( ) ( ) x + y + z + α PPP x y z PPP y z x PPP z x y 1 + α13ppp xyz ( )( x y z ) ( x y z ) ( x y y z z x ) where ΔG stands for the free energy difference of ferroelectric phase and that of paraelectric phase, P x, P y, and P z are the components of the polarization vector in the x, y, and z directions respectively. The coefficients, α i,α ij,α ijk must be consistent with the crystal symmetry. To investigate domain formation and other phenomena in ferroelectrics, these equations are often used in the context of a phase field model. Typically, this involves adding a gradient term, an electrostatic term and an elastic term to the free energy. In all known ferroelectrics, α 0 and α 111 are of positive values. These coefficients may be obtained experimentally or from abinitio simulations. For ferroelectrics with a first order phase transition, α 11 is negative, and α 11 is positive for a second order phase transition. The ferroelectric properties for a cubic to tetragonal phase transition may be obtained by considering the one dimension expression of the free energy which is: Δ G= α0 ( T T0 ) Px + α 11Px + α 111Px () 4 6 The shape of above free energy is schematically shown in Fig. 1 at different temperatures for first order phase transitions. In the following numerical calculations, parameter values are set as α 0 =1, T 0 =1, α 11 =1and α 111 =1 in arbitrary unit for simplicity. (1) Fig. 1. Free energy for a first order ferroelectric phase transition at different temperatures There are four characteristic temperatures in the phase transition process, i.e., CurieWeiss temperature T 0, Curie temperature T c, ferroelectric limit temperature T 1 and limit temperature
3 Theories and Methods of First Order Ferroelectric Phase Transitions 77 of field induced phase transition T. The CurieWeiss temperature can be easily accessed experimentally from the CurieWeiss law of dielectric constant ε at paraelectric phase, i.e., C ε p = TT 0 (3) In above expression, C is the CurieWeiss constant, subscript p of ε stands for paraelectric phase. However the Curie temperature is less accessible experimentally. This temperature measures the balance of the ferroelectric phase and the paraelectric phase. At this temperature, the free energy of ferroelectric phase is the same as that of paraelectric phase. When temperature is between T 0 and T c, ferroelectric phase is stable and paraelectric phase is metastable, this can be easily seen in Fig.1. When the temperature is between T c and T 1, ferroelectric phase is in metastable state while paraelectric phase is stable. When the temperature is higher than T 1, ferroelectric phase disappears. Normally, this temperature is corresponding to the peak temperature of dielectric constant when measured in heating cycle. In other words, peak temperature of dielectric constant measured in heating cycle is the ferroelectric limit temperature T 1, not the Curie temperature T c in a more precise sense. Between temperature T 1 and T, ferroelectric state still can be induced by applying an external electric field. The polarization versus the electric field strength is a double hysteresis loop, which is very similar with that observed in antiferroelectric materials. When the temperature is higher than T, only paraelectric phase can exist. The characteristic temperatures T c, T 1 and T can be easily determined from Eq.() of free energy as following. The Curie temperature T c can be obtained from the following two equations; Δ G= α0( Tc T0) Px + α 11Px + α 111Px = 0 (4) 4 6 Δ G = α 3 5 ( TTP ) +α P +α P = P x 0 c 0 x 11 x 111 x 0 The first equation means that the free energy of ferroelectric phase is same as that of paraelectric phase, and the second equation implies that the free energy of ferroelectric phase is in minimum. From above two equations, we can have the expression of the Curie temperature T c as (5) 3 α TT c = α α (6) At the ferroelectric limit temperature T 1, free energy has an inflexion point at Ps, the spontaneous polarization. As can be seen from Fig. 1, when temperature is below T 1, free energy has are three minima, i.e., at P=±Ps, and P=0. Above temperature T 1, there is only one minimum at P=0. The spontaneous polarization can be obtained from the minimum of the free energy as, Δ G = α ( TTP 0 ) x +α 11Px +α 111Px = 0 P x ( ) 4 Px α0t T0 +α 11Px +α 111Px = 0 (7)
4 78 Ferroelectrics Since P x = 0 corresponds to a free energy maxima in the ferroelectric phase, the spontaneous polarization Ps is obtained from the solution of the equation: which is 4 ( TT ) P P α +α +α = (8) x 111 x 0 1 P = α ± α 4α α ( T T ) x α 111 (9) Hence at temperature T 1, we have In a more explicitly form, ( TT ) α 4α α = 0 (10) α11 TT 1 = 0 + (11) 4 α α Between temperature T 1 and T, there are still inflexion points, which means ferroelectric phase can be induced by an external electric field. When temperature is above T, the inflexion points disappear. By taking the second derivative of the free energy Eq.(), we can have the solution of the inflexion points, G Δ = α 4 0( TT 0) + α 11P + α x 111P = x Px 1 Px = 3α ± 3α 0α α 10α 111 ( ) ( T T ) (1) (13) That is the polarization at the inflexion points. The limit temperature of the induced phase transition T can be determined by or ( ) ( TT ) 3α 0α α = 0 (14) α TT = α α (15) The temperature dependence of the spontaneous can be calculated from Eq.(9) by elimination of solutions yielding a negative square root (for either the first or second order phase transitions) gives: Px 1 = α ± α 4α α α 111 ( T T ) (16) The temperature dependence of the spontaneous polarization from above equation is shown in Fig.. The four characteristic temperatures are denoted by light arrows. The dark arrows
5 Theories and Methods of First Order Ferroelectric Phase Transitions 79 indicate the temperature cycles. Theoretical temperature hysteresis is ΔT=T 1 T 0. Experimentally, the temperature hysteresis could be larger than this value because of the polarization relaxation process. The hysteresis loop (P x versus E x ) may be obtained from the free energy expansion by adding an additional electrostatic term, E x P x, as follows: Δ G= α0 ( T T0 ) Px + α 11Px + α111px EP x x (17) 4 6 Δ G = α 3 5 ( TTP ) +α P +α P E = P x 0 0 x 11 x 111 x x 0 (18) ( ) 3 5 E =α TTP +α P +α P (19) x 0 0 x 11 x 111 x Fig.. Temperature dependence of the spontaneous polarization Plotting E x as a function of P x and reflecting the graph about the 45 degree line gives an 'S' shaped curve when temperature is much lower than the transition temperatures, as can be seen from curves in Fig. 3. The central part of the 'S' corresponds to a free energy local maximum, since the second derivative of the free energy ΔG respect polarization P x is negative. Elimination of this region and connection of the top and bottom portions of the 'S' curve by vertical lines at the discontinuities gives the hysteresis loop. Temperatures are labeled by each curve, label of 0.7T 0 in Fig. 3 is for temperature T=0.7T 0, and 1.T is for T=1.T, T 1 stands for T=(T 1 +T )/. When the temperature is below Curie temperature T c, normal ferroelectric hysteresis loops can be obtained. When the temperature is between T 1 and T, double hysteresis loop or pinched loop could be observed. That means ferroelectric state is induced by the applied electric field. When the temperature is higher than T, the polarization versus electric field becomes a nonlinear relation, see 1.T curve in Fig. 3. It should point out that curves in Fig. 3 are obtained under static electric field. Experimental
6 80 Ferroelectrics measurements usually are performed using time dependent electric field, mostly in sine form. Therefore the hysteresis loops obtained experimentally might be different from the shapes shown in Fig. 3. Fig. 3. Static hysteresis loops at different temperatures Dynamic behavior of ferroelectrics from theoretical simulation could be more helpful for understanding the experimental observing. The dynamic property of ferroelectrics can be studied using LandauKhalantikov equation (Blinc & Zeks, 1974) dp δδg = Γ (0) dt δ P where Γ is the coefficient of thermodynamic restoring force. This equation has been employed to investigate the switching characters of asymmetric ferroelectric films (Wang et al., 1999) and the effects of external stresses on the ferroelectric properties of Pb(Zr,Ti)TiO 3 thin films (Song et al., 003). By inserting free energy (17) into Eq.(0), we have dp 3 5 = Γ α ( ) +α +α dt 0 TTP 0 x 11Px 111Px Ex (1) From above equation, hysteresis loops at different temperature and frequency can be obtained with the electric field is in sine form, Ex = E0 sin( ω t) () The hysteresis loops showing in Fig. 4 are at Curie temperature T c, T 1, (T 1 +T )/, T and 1.T with frequency ω=0.001, E 0 =0.5 and Γ=.0. At Curie temperature T c, a normal ferroelectric hysteresis loop is obtained. At temperature T 1, the hysteresis loop is pinched. Between T 1 and T, double hysteresis loop is obtained as expected, see the blue curve in Fig. 4 for temperature T= (T 1 +T )/. However, at temperature T, double hysteresis loop can be
7 Theories and Methods of First Order Ferroelectric Phase Transitions 81 still observed because of the finite value of relaxation time. Higher than T, no hysteresis can be observed, but a nonlinear PE relation curve. Similar shapes of hysteresis loops have been observed in Pb x Sr 1x TiO 3 ceramics recently(chen et al., 009). Fig. 4. Dynamic hysteresis loops at different temperatures with frequency ω= Dark loop is at Curie temperature T c, red curve is for T 1, blue curve for (T 1 +T )/, green curve for T, and dark line for T=1.T. To get insight understanding of the influence of the frequency on the shape of the hysteresis, more hysteresis loops are presented in Fig. 5. The frequency is set as ω=0.001 for green curves, ω=0.01 for red curves and ω=0.03 for blue curves at Curie temperature T c, T 1, (T 1 +T )/ and at T respectively. At Curie temperature T c, see Fig. 5(a), the coercive field increases with increasing of measure frequency, but the spontaneous polarization is less influenced by the frequency. At temperature T 1, this temperature corresponding to the peak temperature of dielectric constant when measured in heating cycle, pinched hysteresis loop can be observed at low frequency, see the green curve in Fig. 5(b). At higher frequency, the loop behaves like a normal ferroelectric loop, see blue curve in Fig.5(b). When temperature is between T 1 and T, as shown in Fig. 5(c) for temperature at T=(T 1 +T )/, typical double hysteresis loop can be observed at low frequency. When the frequency is higher, it becomes a pinched loop. This trend of loop shape can be kept even when temperature is up to T, see curves in Fig. 5(d). Temperature dependence of polarization at different temperature cycles can be also obtained from Eq.(1) with a constant electric field E=0.01. The results are shown in shown in Fig. 6 with different Γ, the coefficient of thermodynamic restore force. The dark line is for the static polarization, red curves are field heating, blue curves are field cooling. Solid lines are for Γ=100, and dashdotted lines are for Γ=10. The temperature hysteresis from the static theory, as indicated by the two dark dash lines, is smaller than that from Landau Khalanitkov theory. In other words, temperature hysteresis ΔT measured experimentally would be usual larger than that from static Landau theory. Also the temperature hysteresis ΔT depends on Γ, since Γ is related with the relaxation time. A larger Γ represents small
8 8 Ferroelectrics relaxation time, or quick response of polarization with electric field. Hence ferroelectrics with long relaxation time, i.e., small Γ, would expect a very larger temperature hysteresis. Fig. 5. Hysteresis loops with frequency ω=0.001 for green curves, ω=0.01 for red curves and ω=0.03 for blue curves at temperature (a) T c ; (b) T 1 ; (c) (T 1 +T )/, (d) T Fig. 6. Temperature dependence of polarization at different temperature cycles. Dark line is for the static polarization. Red curves are field heating, blue curves are field cooling. Solid lines are for short relaxation time(larger Γ), and dashdot lines are for lone relaxation time (small Γ).
9 Theories and Methods of First Order Ferroelectric Phase Transitions Effective field approach The effective field approach has proved to be a simple statistic physics method but valuable way to describe phase transitions (Gonzalo, 006). The main supposition of this model is that each individual dipole is influenced, not only by the applied electric field, but by every dipole of the system. In its simplest form, which takes into account only dipole interactions, describes fairly well the main features of continuous ferroelectric phase transitions, i.e. second order phase transition. The inclusion of quadrupolar and higher order terms into the effective field expression is necessary for describing the properties of discontinuous or first order phase transitions (Gonzalo et al., 1993; Noheda et al., 1993, 1994). The effective field approach has turned out to be successful explaining the composition dependence of the Curie temperature in mixed ferroelectrics systems (Ali et al., 004; Arago et al., 006). A quantum effective field approach has also been developed for phase transitions at very low temperature (Gonzalo, 1989; Yuan et al., 003; Arago et al., 004) in ferroquantum paraelectric mixed systems. In this section, quantum effective field approach is adopted to reveal the influence of the zero point energy on first order phase transitions (Wang et al., 008). We can see that when the zero point energy of the system is large enough and the ferroelectric phase is suppressed, a phase transitionlike temperature dependence of the polarization can be observed by applying an electric field. The effective field, as described in detail in Gonzalo s book (Gonzalo, 006), can be expressed as E E P P P 3 5 eff = +β +γ +δ + (3) where E is the external electric field, and the following terms correspond to the dipolar, quadrupolar, octupolar, etc., interaction. By keeping the first two terms, i.e. dipolar and quadrupolar interaction, gives account of the first order transition. From statistical considerations, the equation of state is, 3 Eeff μ ( EPP + β +γ ) μ PN = μ tanh = Nμtanh kt B kt B where N is the number of elementary dipoles per unit volume, μ is the electric dipole moment, k B is the Boltzmann constant, and T is the absolute temperature. The Curie temperature is given by βnμ TC = k The explicit form of the equation of state can be rewritten from Eq.(4), kt B P E = tanh βpp γ μ Nμ B 1 3 In order to handle easier this expression, following normalization quantities are introduced, E P T kt γn μ e p t = g B ; ; ; βnμ Nμ TC βnμ β (4) (5)
10 84 Ferroelectrics so Eq. (5) is rewritten as or 3 p tanh epg + + p = t (6) et 1 3 = tanh ppgp (7) and as in absence of external field e = 0, p = p S ps + gp t = (8) tanh 3 S 1 ps Fig.7 shows the plot of the normalized spontaneous polarization p S versus normalized temperature t obtained from Eq. (8) for several values of the parameter g. As it is shown in the discussion of the role of the quadrupolar interaction in the order of the phase transition (see Gonzalo et al., 1993; Noheda et al., 1993; Gonzalo, 006), values of g smaller than 1/3 correspond to a second order, or continuous phase transition, and values larger than 1/3 indicate that the transition is discontinuous, that is, first order. In this case, a spontaneous polarization p θ exists at temperature T θ >T C, and then τ θ >1, being Δt = t θ 1 the corresponding reduced thermal hysteresis, which is the signature of the first order transitions. Fig. 7. Temperature dependence of the spontaneous polarization for different quadrupolar interaction coefficient g. The inset shows the polarization discontinuity p θ (g) and the thermal hysteresis temperature Δt(g) in a first order transition.(wang et al., 008) In order to determine p θ (g), deriving in Eq. (8), t p S pθ = 0
11 Theories and Methods of First Order Ferroelectric Phase Transitions 85 and p θ (g) can be obtained from ( p )( gp ) 1 p ( p gp 3 θ θ θ θ θ) tanh + = 0 (9) Substituting p θ (g) in Eq. (8) again we obtain t θ (g). The inset of Fig.7 shows p θ (g) and Δt(g) respectively. It can be seen that Δt grows almost linearly with g and that p θ approaches to a saturation value that, resolving Eq.(9), turns out to be p θ = when g. When a phase transition takes place at very low temperature it is necessary to consider quantum effect. The energy of the system is no longer the classical thermal energy k B T, but the corresponding energy of the quantum oscillator, 1 E = ω 0 + n being E 0 = ħω 0 / the zero point energy, and <n> the average number of states for a given temperature T. From this quantum energy expression we can obtain a new temperature scale T Q (see Arago et al., 004) defined as, 1 1 Q Q ω0 ω 0 + kt 0 / kt B T ω B e 1 k tanh /kt B ( ω ) and then, the corresponding quantum normalized temperature, t Q T Q /T C. If we introduce a new normalization for the zero point energy so we can rewrite, E ω / Ω 0 0 kt = β BC N μ 0 B (30) Q t and Eq. (7) and (8) become respectively, Ω tanh / ( Ω t ) (31) Q 1 3 = (3) et tanh ppgp t Ω p + gp =, e = Q S S tanh ( Ω / t) tanh ps The temperature dependence of the spontaneous polarization can be found from above equation for a given value of g and different values of the parameter Ω. Fig. 8 plots p S (t) with g = 0.8 to ensure it is a first order transition. The influence of the zeropoint energy is quite obvious: when it is small, the phase transition is still of normal first order one. As the zero point energy increases, both the transition temperatures and the spontaneous polarization decrease. The Curie temperature goes to zero for Ω = 1, but no yet t θ, neither the saturation spontaneous polarization does. From the definition of the normalized zero point energy Ω, we can see then that the Curie temperature goes to zero when the zero point energy is the same as the classical thermal energy k B T C. Imposing again the condition of the zero slope, (33)
12 86 Ferroelectrics ( t/ p S )p θ = 0, we can obtain p θ (Ω), and then t θ (Ω), which must be zero when the ferroelectric behavior will be completely depressed. In this way we work out the zero point energy critical value (Ω cf = for g=0.8) that would not allow any ordered state. Furthermore, from the condition t θ (Ω cf, g) = 0, we will find the relationship between the critical zero point energy Ω cf and the strength of the quadrupolar interaction given by the coefficient g. Fig. 9 plots Ω cf (g) that indicates that Ω cf grows almost linearly with g, specially for larger values of g. This means that ferroelectrics with strong first order phase transition feature needs a relative large critical value of zero point energy to depress the ferroelectricity. Fig. 8. Temperature dependence of the spontaneous polarization at different zero point energy. All curves correspond to a quadrupolar interaction coefficient g=0.8. (Wang et al., 008) Above results prove that a ferroelectric material, with strong quadrupolar interaction, undergoes a first order transition (g>1/3) unless its zero point energy reaches a critical value, Ω cf, because in such case the phase transition is inhibited. However, an induced phase transition must be reached by applying an external electric field. Let be a system with g= 0.8, and Ω=1.6, that is a first order ferroelectric with a zero point energy above the critical value and, hence, no phase transition observed. And let us apply a normalized electric field e that will produce a polarization after Eq. (3). Fig. 10 plots p(t) for different values of the electric field. It can be seen that when it is weak (see curves corresponding to 0.01 and 0.0), the polarization attains quickly a saturation value, similar to what is found in quantum paraelectrics. The curve of e=0.03 (see the dashed line) is split into two parts. The lower part would represent a quantum paraelectric state, but the upper part stands for a kind of ferroelectric state. Therefore there exists a critical value between e=0.0 and 0.03, which is the minimum electric field for inducting a phase transition. For 0.04<e<0.06 the induced polarization curve shows a discontinuous step, but as the electric field increases, 0.07, 0.08 and so on, the polarization changes continuously from a large value at low temperature to a relative small value at high temperature, showing a continuous step. So there is another critical electric field somewhere in between 0.05<e<0.07, separates the discontinuous step
13 Theories and Methods of First Order Ferroelectric Phase Transitions 87 and the continuous step of the induced polarization. In fact, this tricritical point would be around e=0.06. It is also important to remark that the abovementioned features of the field induced phase transitions have been observed in lead magnesium niobate (Kutnjak et al., 006), which is a wellknown ferroelectric relaxor. Fig. 9. Quadrupolar interaction dependence of the critical zero point energy Ω cf that depress ferroelectricity. (Wang et al., 008) Fig. 10. Temperature dependence of the field induced polarization for Ω=1.15 and g=0.8. The parameter is the strength of the electric field. (Wang et al., 008)
14 88 Ferroelectrics For further understanding the field induced phase transitions, Fig. 11 shows the hysteresis loops obtained numerically from Eq. (3) and corresponding to the curves displayed in Fig. 10. Double hysteresis loops can be observed when the temperature is lower than a critical point, around t=0.6, suggesting that ferroelectricity can always be induced at very low temperature. When the temperature is higher than this critical value, there is no hysteresis loop and we can just observe a nonlinear p e behaviour (see for instance the case for t=0.7). However, when the electric field is lower than e 0.05, as indicated by the dashed arrow in Fig. 11, no hysteresis loop can be observed. That is the case corresponding to the curves e =0.01 and 0.0 in Fig. 10. The critical electric field able to induce a phase transition logically increases with the increasing of temperature, so at lower temperature region in Fig. 10, we can always have field induced ferroelectricity when the applied electric field is strong enough. Fig. 11. Hysteresis loops at different temperatures for Ω=1.15 and g=0.8. The dashed arrow indicates the minimum electric field needed to induce a ferroelectric state at t=0. (Wang et al., 008) To understand the influence of the zero point energy on the shape of hysteresis loop, here we take the case of g=0.8 at t=0 as example. The corresponding quantum temperature, after Eq. (31), is and then, Eq. (3) becomes Q tt ( = 0) =Ω e 1 3 =Ωtanh ppgp (34) Fig. 1 plots the hysteresis loops calculated after Eq. (34). When the zero point energy is smaller than the critical value Ω cf (Ω cf =1.136, in this case) a normal hysteresis loop is obtained, where the coercive field decreases as zero point energy increases. For the critical value, a double hysteresis loop with zero coercive field is found. But if we continue
15 Theories and Methods of First Order Ferroelectric Phase Transitions 89 increasing the zero point energy, we arrive to a point where no hysteresis loop is found at all. That suggests that above this other critical value, be Ω cp, there is no way to induce a phase transition, even applying a strong field, and the system remains always in a paraelectric state. Fig. 1. Hysteresis loops at zero temperature for different zero point energy values. The critical value of Ω cf is the minimum zero point energy for the system to have ferroelectricity, while the critical value of Ω cp is the maximum zero point energy for the system to get field induced ferroelectricity. (Wang et al., 008) From the analysis of the hysteresis loops in Fig.1 we can determine the critical electric field needed to induce phase transition imposing the conditions, and deriving in Eq. (34) we get, e e = 0, > 0 p p p c hence we obtain, Ω Ω gp = g p > 1 p ( 1 pc ) 1 3 c 0, 6 0 c c (35) ( 3g 1) + ( 3g 1) 6g( Ω ) pc 6g = (36) Substituting p c (g, Ω) obtained after Eq. (36) into Eq. (34) we can get the coercive field e c (p c ) at zero temperature. Besides, as it is showed in Fig. 1, when the zero point energy attains its critical value Ω cf, the coercive field turns out to be zero, so this is another way to check
16 90 Ferroelectrics the quadrupolar interaction dependence of the critical zero point energy Ω cf (g) as displayed in Fig.9. It must be noted the full accordance between the two calculations. At the second critical value of the zero point energy, Ω cp, the hysteresis loop becomes an inflexion ep curve as it can also be observed in Fig.1, so in this case both Eq. (35) must be equal to zero, and by solving the system of equations, it results, ( g ) g 1 Ω cp =, pcp = (37) 1g 6g The phase diagram at zero temperature is shown in Fig. 13. It displays the role of both the quadrupolar interaction strength and the zero point energy on first order phase transitions. On the top of this diagram we find just paraelectric state (PE), while on the bottom left it appears only second order phase transitions (FE: nd order) that correspond to g < 1/3 and Ω 1. On the bottom right (g > 1/3) there are the first order transitions (FE: 1st order) as the critical values of the zero point energy (Ω cf >1) that depress the ferroelectricity grow monotonously with g. Above the curve Ω cf (g) there are induced electric field phase transitions (first order also). They are limited by another curve Ω cp (g) given by Eq. (37) indicating that no phase transition can be observed when the zero point energy of the system is greater than this value. Fig. 13. Phase diagram of zero point energy critical value Ω c versus quadrupolar interaction coefficient g at zero temperature. The second order phase transition region is denoted as FE:nd order, FE:1st order indicates a normal first order transition, ife is the region of induced ferroelectric phase and on the top, PE corresponds to the paraelectric phase. (Wang et al., 008) From above calculations in the framework of effective field approach, it can be seen that a phase transition can be induced by applying an electric field in a first order quantum paraelectric material. There exist two critical values of the zero point energy, one is Ω cf that depress ferroelectricity, and another is Ω cp above which it is impossible to induce any kind
17 Theories and Methods of First Order Ferroelectric Phase Transitions 91 of phase transition independently of the value of the electric field applied. Phase diagram is presented to display the role of both the quadrupolar interaction strength and the zero point energy on the phase transitions features. 4. Ising model with a fourspin interaction Ising model in a transverse field with a fourspin interaction has been used to study the firstorder phase transition properties in many ferroelectric systems. Under the meanfield approximation, firstorder phase transition in ferroelectric thin films (Wang et al., 1996; Jiang et al., 005) or ferroelectric superlattices (Qu, Zhong & Zhang, 1997; Wang, Wang & Zhong, 00) have been systematically studied. Using the Green s function technique, the firstorder phase transition properties in orderdisorder ferroelectrics (Wang et al., 1989) and ferroelectric thin films (Wesselinowa, 00) have been investigated. Adopting the higherorder approximation to the Fermitype Green s function, the firstorder phase transition properties have been studied in the parameter space with respect to the ratios of the transverse field and the fourspin interaction to the twospin interaction for ferroelectric thin films with the uniform surface and bulk parameters (Teng & Sy,005). These works prove that Ising model with fourspin interaction is a successful model for studying first order phase transition of ferroelectrics. In the following, basic formulism under meanfield approximations and Monte Carlo simulation are presented, and the results are discussed. 4.1 Mean field approximation The Hamiltonian of the transverse field Ising model with a fourspin interchange interaction term is (Wang et al., 1989; Teng & Sy, 005): (38) x ( ) zz ( 4) zzzz ii ij i j ijkl i j kl i ij, ijkl,,, H = ΩS J SS J SSSS where Ω is the transverse field, S x and S z are the x and z components of pseudospin1/ operator, J () and J (4) are the twospin and fourspin exchang interaction, subscript i,j,k,l are site number, summation run over only the nearestneighbor sites. Under the mean field approximation (Blinc & Zeks,1974), solutions of Hamiltonian Eq.(38) is, where x F Ω i Si = tanh Fi kt B y Si = 0 z 4 z 3 JSi + J Si + μe z F i Si = tanh Fi kt B For a homogenous system z 4 z z z Fi = Ω + JS ij j + JijklSSS j k l μe < ij> < ijkl>
18 9 Ferroelectrics S = S = S = S = S z z z z z i j k l J = J J = J F = F j 4 ij, ' ijkl, i jkl Therefore we have, ' 3 z JR + JR + μe F RS = i = tanh F kt B (39) ( ' ) 3 F JR J R E The polarization is related to the zcomponent spin average as, = Ω μ (40) z P = NS μ = NR μ (41) Following normalizations are introduced to handle easier this expression, J' Ω 4kT B F 4μE P g ' =, ω=, t =, τ=, e=, p= = R J J J J J Nμ Eq.(39) and (40) can be rewritten as, i ' pgp + 3 /4+ e τ p = tanh τ t (4) p p 3 e τ= ω + + g + ' 8 In the absence of transverse field, i.e., ω=0 in Eq.(43), and by defining quadrupolar contribution factor g as, 4 g ' J g = = 4 4 J Eq.(4) can be rewritten in the same form in Eq. (6), which is obtained from effective field approach. The equivalence of effective field approach and Ising model with four spin couplings under mean field approximation is completely approved. Therefore the critical value of relative quadrupolar contribution is g c =1/3 under mean field approximation for occurrence of first order phase transition. (43) 4. Monte Carlo simulation A well known and useful method to study phase transitions is by means of the Monte Carlo simulations (Binder, 1984). In particular, phase transitions in Ising systems of relatively low dimensions are sufficient to carry out numerical simulations in the vicinity of the transition temperature, providing a good empirical basis to investigate the asymptotic behavior at the phase transition (Gonzalo & Wang, 008). Here Monte Carlo simulation is applied to the
19 Theories and Methods of First Order Ferroelectric Phase Transitions 93 Ising model with fourspin coupling for studying the phase transition behavior, especially checking the critical value from the fourspin coupling strength, or quadrupolar contribution (Wang et al., 010). Monte Carlo method with metropolis algorithm has been used to simulate 3D Ising cubic lattice. The Hamiltonian is same as in Eq.(38), but without the first term, i.e., without including the tunneling term. In this case, the critical value of the fourspin coupling contribution under mean field approximation is 1 J' J' 1 g = c, ( J '/ J) c 1/6 J = J = 3 = The critical fourspin coupling strength is J /J=1/6 from mean field theory, which is a reference value for the Monte Carlo simulations. Periodic boundary condition has been used in the simulations. The lattice size is denoted as N=L L L, where L is edge length. In the Monte Carlo simulation, edge length L=0, 30, 100 are used. Monte Carlo steps are chosen different for different lattices size to achieve an adequate accurate of the results. Fig. 14. Temperature dependence of spin average (a) and reduced average energy of cubic lattice with edge length L=0 and 30 for different fourspin coupling strength J /J. (Wang et al., 010) Simulation is started with relative small lattice size, with edge length L=0 and 30. The temperature dependence of the spin average and the reduced average energy with different fourspin coupling strength are presented in Fig.14. The reduced average energy is defined as the energy with respective to the ground state energy E 0 in the temperature of zero Kelvin. The curve for lattice size L=0 is marked by solid symbols, and that for L=30 is marked by open symbols. The temperature is in the scale of twosite coupling J. As the fourspin coupling strength increases from J /J =0 to J /J =1, the transition temperature is shifted to higher temperature. The decreasing of the average spin and the increasing of the reduced average energy, with increasing temperature around the transition temperature becomes more rapidly as J /J increases. The general difference between L=0 and that of L=30 is marginal except around the transition temperatures. Even though the fourspin coupling
20 94 Ferroelectrics strength (J /J) is much larger than that of the mean field value 1/6, the first order transition characteristic is not such obvious in these two lattice sizes. The temperature dependence of spin average and the reduced average energy of lattice size 100 is shown in Fig.15 for different fourspin coupling strength J /J. The value of J /J increases from 0.0 to 1.1 with increment of 0.1, corresponding the curves from left to right. The general behavior seems similar with that for L=0 and 30 as shown in Fig.14. However, with increasing of the fourspin coupling strength J /J, as can be seen in the most right side curve of J /J=1.1 in Fig.15(a), the spin average drops down around the transition temperature very quickly, showing a discontinuous feature. Similar discontinuous feature can be also seen in the reduced average energy curves in Fig.15(b). The reduced average energy goes up very sharply around the transition temperature for J /J=1.1, as shown in the most right side curve in Fig.15(b). From Fig.15(b), we also notice that there is an inflexion point around the transition temperatures. The reduced average energy at this point is about 1/3 of the ground state energy when J /J is larger. This condition could supply a criterion for determine the transition temperature in the first order phase transition. Fig. 15. Temperature dependence of spin average (a) and reduced average energy (b) of lattice size L =100 for with different fourspin coupling strength J /J. (Wang et al., 010) To determine the transition temperature, we appeal the calculation of the Binder cumulant. The temperature dependence of the Binder cumulant for J /J= 1.0 with different lattice size are shown in Fig.16. For lattice size of L=10, 0, 5, 30 and 40, the Binder cumulant does cross the point at T c =8.148J. For lattice size L is larger, see L= 50, 70, 100 and 150, the Binder cumulant misses the cross point, and drops down from /3 to a very small value at higher temperatures. That means that the transition temperature can not be obtained from the Binder cumulant when the fourspin coupling strength J /J is larger. It is believed that the Binder cumulants in Fig.16 suggesting the transition is of second order when the lattice size is smaller than L=40, and the transition is of first order when the lattice size is larger than L=40. The lattice size L=40 is around the critical lattice size for fourspin coupling strength J /J =1. This also implies that the transition temperature of first order transition is lattice size dependent.
21 Theories and Methods of First Order Ferroelectric Phase Transitions 95 Fig. 16. Binder cumulants for J /J= 1.0 with different lattice sizes. The circle indicates the cross point of the Binder cumulants for lattice size L<40. (Wang et al/, 010) Spin Average <S> J '=0. 00 J '=0. 10 J '=0. 0 J '=0. 30 J '=0. 40 J'=0.50 J '=0. 60 J'=0.70 J '=0. 75 J '=0. 80 J '=0. 90 J '=1. 00 J '= Te mperature T/Tc <E>/E Tempe rature T/Tc J'=0.00 J'=0.10 J'=0.0 J'=0.30 J'=0.40 J '=0.50 J'=0.60 J '=0.70 J'=0.75 J'=0.80 J'=0.90 J'=1.00 J'=1.10 Fig. 17. Temperature dependence of spin average of lattice sizes L=100 for different J /J around the transition temperature. Temperature is scaled by the transition temperature determined by the criterion <E>/E 0 =1/3. (Wang et al., 010) Fig.17 shows the temperature dependence of spin average and the reduced average energy of lattice size 100 as shown in Fig.15, but with temperature rescaled by the transition temperature T C. The transition temperature T C is determined by the criterion of the averaged energy being one third of the ground state energy, i.e., temperature at <E>/E 0 =1/3 being the transition temperature, as circled in Fig.17(b). Results from Monte Carlo simulations on Ising cubic lattices with four spin couplings suggest that, (1) critical value of fourspin coupling strength for occurrence of first order
22 96 Ferroelectrics phase transition is larger than that of mean field theory; () the critical value is lattice dependence. When lattice size is smaller, the phase transition is still of second order; (3) when the phase transition is of first order, the transition temperature can be determined by the average energy being a third of the ground state energy. However, this criterion has not been justified rigorously. 5. Ferroelectric relaxors Ferroelectric relaxors have been drawn much attention because of their high electromechanical performance and unusual ferroelectric properties. Two review articles (Ye, 1998; Bokov & Ye, 006) have summarized the achievements of recent researches on ferroelectric relaxors, especially for lead magnesium nibate (PMN). Basically, there are two categories of explanations about the fundamental physics of their unusual properties. One is based upon the randomness of their compositions and structures, such as Smolenskii s theory and spherical random bond random field model. Another is presumably based upon the experimental phenomenon, such as macromicrodomain and superparaelectric model. In this section, a general explanation of the properties observed in ferroelectric relaxors is proposed after analysis of the later category models (Wang et al., 009). Field induced phase transition and diffused phase transition are reproduced within the framework of effective field approach. Interpretation is started with the experimental results of field induced phase transition in PMN. The temperature dependence of the polarization under different electric field strengths has been obtained (Ye & Schmid, 1993; Ye, 1998). From this relation we can understand that (1) there is no ferroelectric phase transition in the whole temperature range, since there is no spontaneous polarization as the temperature goes down to zero Kelvin; () ferroelectricity can be induced by an external electric field. These imply that the phase transition in PMN is of first order, but the ferroelectricity is depressed in the whole temperature range. To understand these characteristics of ferroelectric relaxors, we can recall the temperature dependence of the spontaneous polarization in a typical normal first order ferroelectric phase transition is shown in Fig.. This implies that PMN is in a paraelectric state, but not far from the ferroelectric state. Apart from the field induced phase transition, the following features should be also found within this temperature range in a normal first order ferroelectric phase transition: (1) a very long relaxation time, because of the critical slow down as the temperature is near the critical temperature. () superparaelectric behavior. Normally there should be a double hysteresis loop observed in this temperature range. However, the double hysteresis loop could be reduced to a superparaelectric shape because of the long relaxation time of the critical slow down. (3) macromicrodomain crossover. As the temperature is much lower than the critical temperature, single domain or macrodomain is expected since it is in ferroelectric state; as the temperature is much higher than the critical temperature, no domain will be observed as it is in paraelectric state. Around the critical temperature, macromicrodomain crossover is expected, i.e., polar nanoregions are forming in this temperature range. All these features have been observed in the ferroelectric relaxors like PMN. The depression of the ferroelectricity in PMN reminds us of the case of quantum paraelectrics SrTiO 3. Therefore the field induced phase transition in a first order phase transition depressed by quantum fluctuation has been investigated within the framework of effective field approach by inclusive of zero point energy (Wang et al., 008). The
23 Theories and Methods of First Order Ferroelectric Phase Transitions 97 temperature dependence of the induced polarization under different electric field is shown in Fig.10. The polarization p and temperature t are in dimensionless unit, the numbers marked in the Fig.10 are the strength of electric field. The major difference between the temperature dependence of the polarization in PMN (Ye & Schmid, 1993; Ye, 1998) and Fig.10 appears at lower temperature range. The polarization of PMN is still difficult to recover by an external field. This suggests that the zero point energy at lower temperature could be much larger than that in the higher temperature. In other words, the zero point energy might be increased with decreasing of temperature. Another evidence of the existence of larger zero point energy can be found from the diffused phase transition in PMN. For the quantum temperature scale with constant zero point energy, the temperature dependence of the dielectric constant has been obtained from Monte Carlo simulation on a Ising model (Wang et al., 00). As the zero point increases, the transition temperature or the peak temperature of the dielectric constant shifts to a lower temperature. As the zero point energy is larger than the critical value, quantum paraelectric feature is obtained. When the zero point energy increases further, the dielectric constant decreases at low temperature. Therefore if the zero point energy changes with temperature and has a larger value only at lower temperature, the dielectric constant will increase as the temperature increases at lower temperature side, and decreases as the temperature increases at higher temperature side. A round dielectric peak will be formed around the temperature of zero point energy dropping down. From above analysis, a temperature dependent form of zero point energy is proposed in the following form (Wang et al., 009) ω ω= (44) + 0 ( TTX ) 1 e α where the zero point energy ω changes around temperature T x from ω 0 at lower temperature to a relative lower value with crossover rate α. By using the same technique of effective field approach as in Refs.(Wang et al., 008; Yuan et al., 003 Gonzalo, 006), with the quantum temperature scale in Eq.(3) and the zero point energy in Eq.(44), the field induce phase transition and diffused phase transition are obtained and shown in Fig.18. All parameters are in dimensionless scale, e stands for the electric field, and k is for the dielectric constant. From Fig.18 we can see that the basic features of field induce phase transition and diffused phase transition observed in relaxor ferroelectric are reproduced. Fig. 18. (a) Field induced phase transition and (b) diffused phase transition. (Wang et al., 009)
24 98 Ferroelectrics The dimensionless quantum temperature scale used in Fig.18 is shown in Fig.19. The solid line represents the quantum temperature scale, and the dashed line is for the real temperature scale. The phase transition temperature is marked by the arrow. That means that the state evolution of relaxor ferroelectric misses the phase transition temperature as the temperature decreases, and reentry of the paraelectric state. The kind of nonergodic behavior is schematically shown in Fig.19(b) for better understanding. Fig. 19. (a) Quantum temperature scale and (b) nonergodic behavior. (Wang et al., 009) Overall, relaxor ferroelectrics like PMN are in a tricritical state of long range ferroelectric order, thermal fluctuations and quantum fluctuations. This critical state can be described by a quantum temperature scale. Following features can be understood from this issue: diffuse phase transition, field induced phase transition, long relaxation time, as well as superparaelectric state, micromacrodomain crossover and nonergodic behavior. However, a more adequate expression of temperature dependence of zero point energy is still needed for better description of the physical behavior in the relaxor ferroelectrics. 6. Final remarks Theoretical methods and models for studying ferroelectric with first order phase transition are definitely not limited to the contents in this chapter. Hopefully results from these theoretical techniques can provide useful information for understanding experimental observations. Heavycomputer relying methods, such as firstprinciple calculations and molecular dynamic simulations etc, have been applied to investigate the physical properties of ferroelectrics. However, fully understanding of the origin of ferroelectrics might need more efforts from both theoretical and experimental side. 7. References Ali, R.A.; Wang, C.L.; Yuan, M.; Wang, Y. X. & Zhong, W. L. (004). Compositional dependence of the Curie temperature in mixed ferroelectrics: effective field approach. Solid State Commun., 19, Arago, C.; Garcia, J.; Gonzalo, J. A.; Wang, C. L.; Zhong, W. L. & Xue, X. Y. (004). Influence of quantum zero point energy on the ferroelectric behavior of isomorphous systems. Ferroelectrics, 301,
25 Theories and Methods of First Order Ferroelectric Phase Transitions 99 Aragó, C.; Wang, C. L. & Gonzalo, J. A. (006). Deviations from Vegard s law in the Curie temperature of mixed ferroelectric solid solutions. Ferroelectrics, 337, Binder, K. (1984). Applications of Monte Carlo Method in Statistical Physics, nd Edition, SpringerVerlag, ISBN X, Berlin Blinc, R. & Zeks, B. (1974). Soft modes in ferroelectrics and antiferroeletrics, NorthHolland Publishing Company, ISBN , Amsterdam Bokov, A. A. & Ye, Z. G. (006). Recent progress in relaxor ferroelectrics with perovskite structure. Journal of Materials Science, 41, 315 Chen, H. W.; Yang, C.R.; Zhang, J.H.; Pei, Y.F. & Zhao, Z. (009). Microstructure and antiferroelectriclike behavior of Pb x Sr 1 x TiO 3 ceramics. J Alloys and Compounds, 486, Gonzalo, J. A. (1989). Quantum effects and competing interactions in crystals of the mixed rubidium and ammonium dihydrogen phosphate systems. Phys. Rev. B, 39, Gonzalo, J. A.; Ramírez, R.; Lifante, G. & Koralewski, M. (1993). Dielectric discontinuities and multipolar interactions in ferroelectric perovskites, Ferroelectrics Letters Section, 15, 916 Gonzalo, J. A. (006). Effective Field Approach to Phase Transitions and Some Applications to Ferroelectrics, World Scientific Press, ISBN , Singapore Gonzalo, J. A. & Wang, C. L. (008). Monte Carlo approach to Phase Transitions, Asociacion Espanola Ciencia y Cultura, ISBN ,Madrid Jiang, Q. & Tao, Y. M. (005). Critical line between the firstorder and the secondorder phase transition for ferroelectric thin films described by TIM. Phys. Lett. A, 336, 16 Kutnjak, Z.; Petzelt, J. & Blinc, R. (006). The giant electromechanical response in ferroelectric relaxors as a critical phenomenon. Nature, 441, Lines, M. E. & Glass A. M. (1997). Principles and Applications of Ferroelectrics and Related Materials, Clarendon Press, ISBN , Oxford Noheda, B.; Lifante, G. & Gonzalo, J.A. (1993). Specific heat and quadrupole interactions in uniaxial ferroelectrics, Ferroelectrics Letters Section, 15, Noheda, B.; Koralewski, M.; Lifante, G. & Gonzalo J. A. (1994). Dielectric discontinuities and multipolar interactions in ferroelectric perovskites, Ferroelectrics Letters Section, 17, 531 Qu, B. D.; Zhong, W. L. & Zhang, P. L. (1997). Ferroelectric superlattice with firstorder phase transition. Ferroelectrics, 197, 36 Song, T. K.; Kim, J. S.; Kim, M.H.; Lim, W.; Kim, Y. S. & Lee, J. C. (003). Landau Khalatnikov simulations for the effects of external streese on the ferroelectric properties of Pb(Zr,Ti)O 3 thin films. Thin Soild Films, 44, Teng, B. H. & Sy, H. K. (005). Transition regions in the parameter space based on the transverse Ising model with a fourspin interaction. Europhys. Lett., 7, Wang, C. L.; Qin, Z. K. & Lin, D. L. (1989). First order phase transition in orderdisorder ferroelectrics. Phys. Rev. B, 40, Wang, C. L.; Zhang, L.; Zhong, W. L. & Zhang, P.L. (1999). Switching characters of asymmetric ferroelectric films. Physics Letters A, 54,
Capacitance and Ferroelectrics
Ram Seshadri MRL 2031, x6129 seshadri@mrl.ucsb.edu; http://www.mrl.ucsb.edu/ seshadri/teach.html Capacitance and Ferroelectrics A voltage V applied across a capacitor of caacitance C allows a quantity
More informationPIEZO CERAMICS. Noliac Group develops and manufactures piezoelectric. zirconate titanate (PZT) of high quality and tailored for custom
Noliac Group develops and manufactures piezoelectric zirconate titanate (PZT) of high quality and tailored for custom Piezoelectric components may be used as e.g.: Actuators Sensors Generators Transducers
More informationModern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras
Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras Module  2 Lecture  2 Part 2 of 2 Review of Atomic Bonding II We will continue
More informationEM4: Magnetic Hysteresis
CHALMERS UNIVERSITY OF TECHNOLOGY GÖTEBORG UNIVERSITY EM4: Magnetic Hysteresis Lab manual (version 1.001a) Students:... &... Date:... /... /... Laboration passed:... Supervisor:... Date:... /... /... Raluca
More informationk u (t) = k b + k s t
Chapter 2 Stripe domains in thin films 2.1 Films with perpendicular anisotropy In the first part of this chapter, we discuss the magnetization of films with perpendicular uniaxial anisotropy. The easy
More informationPTC Thermistors [From Philips Data Handbook PA ]
PTC Thermistors [From Philips Data Handbook PA02 1989] 1. GENERAL Positive Temperature Coefficient (PTC) thermistors exhibit a high positive temperature coefficient of resistance. They differ from Negative
More informationBranislav K. Nikolić
Monte Carlo Simulations in Statistical Physics: Magnetic PhaseTransitions in the Ising Model Branislav K. Nikolić Department of Physics and Astronomy, University of Delaware, U.S.A. PHYS 460/660: Computational
More informationElasticity and Equations of State
Elasticity and Equations of State The way planets deform depends primarily upon the elastic properties of the constituent polycrystalline materials. In particular, the speed of body waves passing through
More informationMonte Carlo Simulation
Chapter 4 Monte Carlo Simulation Due to the complexity of the problem, treating irregular spin systems with competing interactions in thermal equilibrium and nonequilibrium, we are forced to use Monte
More informationRecent development in piezoelectric materials used for actuators and sensors applications
Recent development in piezoelectric materials used for actuators and sensors applications Dragan Damjanovic, Ceramics Laboratory, Materials Institute Swiss Federal Institute of Technology  EPFL Lausanne
More informationEXIT TIME PROBLEMS AND ESCAPE FROM A POTENTIAL WELL
EXIT TIME PROBLEMS AND ESCAPE FROM A POTENTIAL WELL Exit Time problems and Escape from a Potential Well Escape From a Potential Well There are many systems in physics, chemistry and biology that exist
More informationElectroceramics Prof. Ashish Garg Department of Materials Science and Engineering Indian Institute of Technology, Kanpur.
Electroceramics Prof. Ashish Garg Department of Materials Science and Engineering Indian Institute of Technology, Kanpur Lecture  30 Again, we start a new lecture. We will just go through the last lecture
More informationElectrical and optical properties of materials
Electrical and optical properties of materials JJL Morton Electrical and optical properties of materials John JL Morton Part 3: Piezo pryo and ferroelectricity We have already seen in the discussion
More informationGlobal Seasonal Phase Lag between Solar Heating and Surface Temperature
Global Seasonal Phase Lag between Solar Heating and Surface Temperature Summer REU Program Professor Tom Witten By Abstract There is a seasonal phase lag between solar heating from the sun and the surface
More informationDetermination of Molecular Weight by Freezing Point Depression
Determination of Molecular Weight by Freezing Point Depression Freezing point depression is a kind of colligative properties as treated in high school chemistry course. Normally used alcohol or mercury
More information7. DYNAMIC LIGHT SCATTERING 7.1 First order temporal autocorrelation function.
7. DYNAMIC LIGHT SCATTERING 7. First order temporal autocorrelation function. Dynamic light scattering (DLS) studies the properties of inhomogeneous and dynamic media. A generic situation is illustrated
More informationElectrochemical Kinetics ( Ref. :Bard and Faulkner, Oldham and Myland, Liebhafsky and Cairns) R f = k f * C A (2) R b = k b * C B (3)
Electrochemical Kinetics ( Ref. :Bard and Faulkner, Oldham and Myland, Liebhafsky and Cairns) 1. Background Consider the reaction given below: A B (1) If k f and k b are the rate constants of the forward
More informationChapter 3: Theory of Paraelectric Capacitance Joe T. Evans, Jr.
Radiant Technologies, Inc. 2835D Pan American Freeway NE Albuquerque, NM 87107 Tel: 5058428007 Fax: 5058420366 www.ferrodevices.com email: radiant@ferrodevices.com Chapter 3: Theory of Paraelectric
More informationMonte Carlo Simulation technique. S. B. Santra Department of Physics Indian Institute of Technology Guwahati
Monte Carlo Simulation technique S. B. Santra Department of Physics Indian Institute of Technology Guwahati What is Monte Carlo (MC)? Introduction Monte Carlo method is a common name for a wide variety
More informationAjit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films
Ajit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films https://cuvillier.de/de/shop/publications/1306 Copyright: Cuvillier Verlag,
More informationNuclear Magnetic Resonance
Nuclear Magnetic Resonance Introduction Atomic magnetism Nuclear magnetic resonance refers to the behaviour of atomic nuclei in the presence of a magnetic field. The first principle required to understand
More informationThe Role of Electric Polarization in Nonlinear optics
The Role of Electric Polarization in Nonlinear optics Sumith Doluweera Department of Physics University of Cincinnati Cincinnati, Ohio 45221 Abstract Nonlinear optics became a very active field of research
More informationUnderstanding Poles and Zeros
MASSACHUSETTS INSTITUTE OF TECHNOLOGY DEPARTMENT OF MECHANICAL ENGINEERING 2.14 Analysis and Design of Feedback Control Systems Understanding Poles and Zeros 1 System Poles and Zeros The transfer function
More informationLong term performance of polymers
1.0 Introduction Long term performance of polymers Polymer materials exhibit time dependent behavior. The stress and strain induced when a load is applied are a function of time. In the most general form
More informationProbability & Statistics Primer Gregory J. Hakim University of Washington 2 January 2009 v2.0
Probability & Statistics Primer Gregory J. Hakim University of Washington 2 January 2009 v2.0 This primer provides an overview of basic concepts and definitions in probability and statistics. We shall
More informationIB Mathematics SL :: Checklist. Topic 1 Algebra The aim of this topic is to introduce students to some basic algebraic concepts and applications.
Topic 1 Algebra The aim of this topic is to introduce students to some basic algebraic concepts and applications. Check Topic 1 Book Arithmetic sequences and series; Sum of finite arithmetic series; Geometric
More informationEffects of node buffer and capacity on network traffic
Chin. Phys. B Vol. 21, No. 9 (212) 9892 Effects of node buffer and capacity on network traffic Ling Xiang( 凌 翔 ) a), Hu MaoBin( 胡 茂 彬 ) b), and Ding JianXun( 丁 建 勋 ) a) a) School of Transportation Engineering,
More informationLecture 3: Electron statistics in a solid
Lecture 3: Electron statistics in a solid Contents Density of states. DOS in a 3D uniform solid.................... 3.2 DOS for a 2D solid........................ 4.3 DOS for a D solid........................
More informationExperiment A5. Hysteresis in Magnetic Materials
HYSTERESIS IN MAGNETIC MATERIALS A5 1 Experiment A5. Hysteresis in Magnetic Materials Objectives This experiment illustrates energy losses in a transformer by using hysteresis curves. The difference betwen
More informationQNET Experiment #06: HVAC Proportional Integral (PI) Temperature Control Heating, Ventilation, and Air Conditioning Trainer (HVACT)
Quanser NIELVIS Trainer (QNET) Series: QNET Experiment #06: HVAC Proportional Integral (PI) Temperature Control Heating, Ventilation, and Air Conditioning Trainer (HVACT) Student Manual Table of Contents
More information4. Thermodynamics of Polymer Blends
4. Thermodynamics of Polymer Blends Polymeric materials find growing applications in various fields of everyday life because they offer a wide range of application relevant properties. Blending of polymers
More informationIncorporating Internal Gradient and Restricted Diffusion Effects in Nuclear Magnetic Resonance Log Interpretation
The OpenAccess Journal for the Basic Principles of Diffusion Theory, Experiment and Application Incorporating Internal Gradient and Restricted Diffusion Effects in Nuclear Magnetic Resonance Log Interpretation
More informationMolecular Dynamics Simulations
Molecular Dynamics Simulations Yaoquan Tu Division of Theoretical Chemistry and Biology, Royal Institute of Technology (KTH) 201106 1 Outline I. Introduction II. Molecular Mechanics Force Field III. Molecular
More informationPrentice Hall Algebra 2 2011 Correlated to: Colorado P12 Academic Standards for High School Mathematics, Adopted 12/2009
Content Area: Mathematics Grade Level Expectations: High School Standard: Number Sense, Properties, and Operations Understand the structure and properties of our number system. At their most basic level
More informationDynamics. Figure 1: Dynamics used to generate an exemplar of the letter A. To generate
Dynamics Any physical system, such as neurons or muscles, will not respond instantaneously in time but will have a timevarying response termed the dynamics. The dynamics of neurons are an inevitable constraint
More informationarxiv:physics/0607202v2 [physics.compph] 9 Nov 2006
Stock price fluctuations and the mimetic behaviors of traders Junichi Maskawa Department of Management Information, Fukuyama Heisei University, Fukuyama, Hiroshima 7200001, Japan (Dated: February 2,
More informationBondcorrelated percolation model and the unusual behaviour of supercooled water
J. Phys. A: Math. Gen. 16 (1983) L321L326. Printed in Great Britain LETTER TO THE EDITOR Bondcorrelated percolation model and the unusual behaviour of supercooled water ChinKun Hu LashMiller Chemical
More informationEffect of coupling strength on magnetic properties of exchange spring magnets
OURNAL OF APPLIED PHYSICS VOLUME 94, NUMBER 10 15 NOVEMBER 2003 Effect of coupling strength on magnetic properties of exchange spring magnets Vamsi M. Chakka, Z. S. Shan a), and. P. Liu b) Department of
More informationFIRST YEAR CALCULUS. Chapter 7 CONTINUITY. It is a parabola, and we can draw this parabola without lifting our pencil from the paper.
FIRST YEAR CALCULUS WWLCHENW L c WWWL W L Chen, 1982, 2008. 2006. This chapter originates from material used by the author at Imperial College, University of London, between 1981 and 1990. It It is is
More informationProbability and Statistics
CHAPTER 2: RANDOM VARIABLES AND ASSOCIATED FUNCTIONS 2b  0 Probability and Statistics Kristel Van Steen, PhD 2 Montefiore Institute  Systems and Modeling GIGA  Bioinformatics ULg kristel.vansteen@ulg.ac.be
More informationCommon Core Unit Summary Grades 6 to 8
Common Core Unit Summary Grades 6 to 8 Grade 8: Unit 1: Congruence and Similarity 8G18G5 rotations reflections and translations,( RRT=congruence) understand congruence of 2 d figures after RRT Dilations
More informationPSS 27.2 The Electric Field of a Continuous Distribution of Charge
Chapter 27 Solutions PSS 27.2 The Electric Field of a Continuous Distribution of Charge Description: Knight ProblemSolving Strategy 27.2 The Electric Field of a Continuous Distribution of Charge is illustrated.
More informationNo Evidence for a new phase of dense hydrogen above 325 GPa
1 No Evidence for a new phase of dense hydrogen above 325 GPa Ranga P. Dias, Ori Noked, and Isaac F. Silvera Lyman Laboratory of Physics, Harvard University, Cambridge MA, 02138 In recent years there has
More information3 Numerical Methods for Convection
3 Numerical Methods for Convection The topic of computational fluid dynamics (CFD) could easily occupy an entire semester indeed, we have such courses in our catalog. The objective here is to eamine some
More informationMETHODOLOGICAL CONSIDERATIONS OF DRIVE SYSTEM SIMULATION, WHEN COUPLING FINITE ELEMENT MACHINE MODELS WITH THE CIRCUIT SIMULATOR MODELS OF CONVERTERS.
SEDM 24 June 16th  18th, CPRI (Italy) METHODOLOGICL CONSIDERTIONS OF DRIVE SYSTEM SIMULTION, WHEN COUPLING FINITE ELEMENT MCHINE MODELS WITH THE CIRCUIT SIMULTOR MODELS OF CONVERTERS. Áron Szûcs BB Electrical
More informationThe Kinetic Theory of Gases Sections Covered in the Text: Chapter 18
The Kinetic Theory of Gases Sections Covered in the Text: Chapter 18 In Note 15 we reviewed macroscopic properties of matter, in particular, temperature and pressure. Here we see how the temperature and
More informationBlasius solution. Chapter 19. 19.1 Boundary layer over a semiinfinite flat plate
Chapter 19 Blasius solution 191 Boundary layer over a semiinfinite flat plate Let us consider a uniform and stationary flow impinging tangentially upon a vertical flat plate of semiinfinite length Fig
More informationCBE 6333, R. Levicky 1. Potential Flow
CBE 6333, R. Levicky Part I. Theoretical Background. Potential Flow Potential Flow. Potential flow is irrotational flow. Irrotational flows are often characterized by negligible viscosity effects. Viscous
More informationSchool of Biotechnology
Physics reference slides Donatello Dolce Università di Camerino a.y. 2014/2015 mail: donatello.dolce@unicam.it School of Biotechnology Program and Aim Introduction to Physics Kinematics and Dynamics; Position
More informationStochastic Doppler shift and encountered wave period distributions in Gaussian waves
Ocean Engineering 26 (1999) 507 518 Stochastic Doppler shift and encountered wave period distributions in Gaussian waves G. Lindgren a,*, I. Rychlik a, M. Prevosto b a Department of Mathematical Statistics,
More informationIn mathematics, there are four attainment targets: using and applying mathematics; number and algebra; shape, space and measures, and handling data.
MATHEMATICS: THE LEVEL DESCRIPTIONS In mathematics, there are four attainment targets: using and applying mathematics; number and algebra; shape, space and measures, and handling data. Attainment target
More informationLecture 4: Thermodynamics of Diffusion: Spinodals
Materials Science & Metallurgy Master of Philosophy, Materials Modelling, Course MP6, Kinetics and Microstructure Modelling, H. K. D. H. Bhadeshia Lecture 4: Thermodynamics of Diffusion: Spinodals Fick
More informationThe factor of safety is a factor of ignorance. If the stress on a part at a critical location (the
Appendix C The Factor of Safety as a Design Variable C.1 INTRODUCTION The factor of safety is a factor of ignorance. If the stress on a part at a critical location (the applied stress) is known precisely,
More informationA boxcovering algorithm for fractal scaling in scalefree networks
CHAOS 17, 026116 2007 A boxcovering algorithm for fractal scaling in scalefree networks J. S. Kim CTP & FPRD, School of Physics and Astronomy, Seoul National University, NS50, Seoul 151747, Korea K.I.
More informationWe consider a hydrogen atom in the ground state in the uniform electric field
Lecture 13 Page 1 Lectures 1314 Hydrogen atom in electric field. Quadratic Stark effect. Atomic polarizability. Emission and Absorption of Electromagnetic Radiation by Atoms Transition probabilities and
More informationHeat Transfer and Energy
What is Heat? Heat Transfer and Energy Heat is Energy in Transit. Recall the First law from Thermodynamics. U = Q  W What did we mean by all the terms? What is U? What is Q? What is W? What is Heat Transfer?
More information6 EXTENDING ALGEBRA. 6.0 Introduction. 6.1 The cubic equation. Objectives
6 EXTENDING ALGEBRA Chapter 6 Extending Algebra Objectives After studying this chapter you should understand techniques whereby equations of cubic degree and higher can be solved; be able to factorise
More informationPlate waves in phononic crystals slabs
Acoustics 8 Paris Plate waves in phononic crystals slabs J.J. Chen and B. Bonello CNRS and Paris VI University, INSP  14 rue de Lourmel, 7515 Paris, France chen99nju@gmail.com 41 Acoustics 8 Paris We
More informationWhen to Refinance Mortgage Loans in a Stochastic Interest Rate Environment
When to Refinance Mortgage Loans in a Stochastic Interest Rate Environment Siwei Gan, Jin Zheng, Xiaoxia Feng, and Dejun Xie Abstract Refinancing refers to the replacement of an existing debt obligation
More informationPURSUITS IN MATHEMATICS often produce elementary functions as solutions that need to be
Fast Approximation of the Tangent, Hyperbolic Tangent, Exponential and Logarithmic Functions 2007 Ron Doerfler http://www.myreckonings.com June 27, 2007 Abstract There are some of us who enjoy using our
More informationDiamagnetism and Paramagnetism. Magnetization M(H) in the presence of an uniform magnetic field H at T=0 is defined as:
Diamagnetism and Paramagnetism Definitions: Magnetization M(H) in the presence of an uniform magnetic field H at T=0 is defined as: where is the ground state energy. Note that H is the magnetic field felt
More informationReview of Fundamental Mathematics
Review of Fundamental Mathematics As explained in the Preface and in Chapter 1 of your textbook, managerial economics applies microeconomic theory to business decision making. The decisionmaking tools
More information3.2 Sources, Sinks, Saddles, and Spirals
3.2. Sources, Sinks, Saddles, and Spirals 6 3.2 Sources, Sinks, Saddles, and Spirals The pictures in this section show solutions to Ay 00 C By 0 C Cy D 0. These are linear equations with constant coefficients
More informationMontana Common Core Standard
Algebra I Grade Level: 9, 10, 11, 12 Length: 1 Year Period(s) Per Day: 1 Credit: 1 Credit Requirement Fulfilled: A must pass course Course Description This course covers the real number system, solving
More information4 Thermomechanical Analysis (TMA)
172 4 Thermomechanical Analysis 4 Thermomechanical Analysis (TMA) 4.1 Principles of TMA 4.1.1 Introduction A dilatometer is used to determine the linear thermal expansion of a solid as a function of temperature.
More informationCation Ordering and Dielectric Properties of PMNPSN Relaxors
Cation Ordering and Dielectric Properties of PMNPSN Relaxors P. K. Davies, L. Farber, M. Valant *, and M. A. Akbas ** Department of Materials Science and Engineering, University of Pennsylvania, Philadelphia,
More informationExperiment #1, Analyze Data using Excel, Calculator and Graphs.
Physics 182  Fall 2014  Experiment #1 1 Experiment #1, Analyze Data using Excel, Calculator and Graphs. 1 Purpose (5 Points, Including Title. Points apply to your lab report.) Before we start measuring
More informationBoring (?) firstorder phase transitions
Boring (?) firstorder phase transitions Des Johnston Edinburgh, June 2014 Johnston First Order 1/34 Plan of talk First and Second Order Transitions Finite size scaling (FSS) at first order transitions
More informationAP Physics 1 and 2 Lab Investigations
AP Physics 1 and 2 Lab Investigations Student Guide to Data Analysis New York, NY. College Board, Advanced Placement, Advanced Placement Program, AP, AP Central, and the acorn logo are registered trademarks
More informationSenior Secondary Australian Curriculum
Senior Secondary Australian Curriculum Mathematical Methods Glossary Unit 1 Functions and graphs Asymptote A line is an asymptote to a curve if the distance between the line and the curve approaches zero
More informationSolution: ΔG = a 3 ΔG v. + 6a 2 γ. Differentiation of this expression with respect to a is as. d ΔG da = d(a3 ΔG v. + d(6a2 γ) = 3a 2 ΔG v.
14:440:407 ch10 Question 10.2: (a) Rewrite the expression for the total free energy change for nucleation (Equation 10.1) for the case of a cubic nucleus of edge length a (instead of a sphere of radius
More informationChapter 24 Physical Pendulum
Chapter 4 Physical Pendulum 4.1 Introduction... 1 4.1.1 Simple Pendulum: Torque Approach... 1 4. Physical Pendulum... 4.3 Worked Examples... 4 Example 4.1 Oscillating Rod... 4 Example 4.3 Torsional Oscillator...
More informationCurrent Standard: Mathematical Concepts and Applications Shape, Space, and Measurement Primary
Shape, Space, and Measurement Primary A student shall apply concepts of shape, space, and measurement to solve problems involving two and threedimensional shapes by demonstrating an understanding of:
More informationFrom transition metal oxides to cosmic strings
From transition metal oxides to cosmic strings (and how electronic structure computations can help) Nicola Spaldin Materials Theory Department of Materials, ETH Zürich Important things that happened as
More information1 Scalars, Vectors and Tensors
DEPARTMENT OF PHYSICS INDIAN INSTITUTE OF TECHNOLOGY, MADRAS PH350 Classical Physics Handout 1 8.8.2009 1 Scalars, Vectors and Tensors In physics, we are interested in obtaining laws (in the form of mathematical
More informationES250: Electrical Science. HW7: Energy Storage Elements
ES250: Electrical Science HW7: Energy Storage Elements Introduction This chapter introduces two more circuit elements, the capacitor and the inductor whose elements laws involve integration or differentiation;
More informationChapter 1: Introduction
! Revised August 26, 2013 7:44 AM! 1 Chapter 1: Introduction Copyright 2013, David A. Randall 1.1! What is a model? The atmospheric science community includes a large and energetic group of researchers
More informationToy Blocks and Rotational Physics
Toy Blocks and Rotational Physics Gabriele U. Varieschi and Isabel R. Jully, Loyola Marymount University, Los Angeles, CA Have you ever observed a child playing with toy blocks? A favorite game is to build
More informationA Theoretical Model for Mutual Interaction between Coaxial Cylindrical Coils Lukas Heinzle
A Theoretical Model for Mutual Interaction between Coaxial Cylindrical Coils Lukas Heinzle Page 1 of 15 Abstract: The wireless power transfer link between two coils is determined by the properties of the
More informationFourier Series. A Fourier series is an infinite series of the form. a + b n cos(nωx) +
Fourier Series A Fourier series is an infinite series of the form a b n cos(nωx) c n sin(nωx). Virtually any periodic function that arises in applications can be represented as the sum of a Fourier series.
More informationFigure 1: (a) Diode cross section. (b) Reverse biased diode. (c) Forward biased diode.
The Junction Diode Basic Operation The diode is fabricated of a semiconductor material, usually silicon, which is doped with two impurities. One side is doped with a donor or ntype impurity which releases
More informationIn a cyclic transformation, where the final state of a system is the same as the initial one, U = 0
Chapter 4 Entropy and second law of thermodynamics 4.1 Carnot cycle In a cyclic transformation, where the final state of a system is the same as the initial one, U = 0 since the internal energy U is a
More informationA wave lab inside a coaxial cable
INSTITUTE OF PHYSICS PUBLISHING Eur. J. Phys. 25 (2004) 581 591 EUROPEAN JOURNAL OF PHYSICS PII: S01430807(04)76273X A wave lab inside a coaxial cable JoãoMSerra,MiguelCBrito,JMaiaAlves and A M Vallera
More informationTechnology of EHIS (stamping) applied to the automotive parts production
Laboratory of Applied Mathematics and Mechanics Technology of EHIS (stamping) applied to the automotive parts production Churilova Maria, SaintPetersburg State Polytechnical University Department of Applied
More informationLecture 3: Introduction to Diffusion
Materials Science & Metallurgy Master of Philosophy, Materials Modelling, Course MP6, Kinetics and Microstructure Modelling, H. K. D. H. Bhadeshia Lecture 3: Introduction to Diffusion Mass transport in
More informationDetailed simulation of mass spectra for quadrupole mass spectrometer systems
Detailed simulation of mass spectra for quadrupole mass spectrometer systems J. R. Gibson, a) S. Taylor, and J. H. Leck Department of Electrical Engineering and Electronics, The University of Liverpool,
More informationSpinlattice and spinspin relaxation
Spinlattice and spinspin relaation Sequence of events in the NMR eperiment: (i) application of a 90 pulse alters the population ratios, and creates transverse magnetic field components (M () ); (ii)
More informationAn analysis of price impact function in orderdriven markets
Available online at www.sciencedirect.com Physica A 324 (2003) 146 151 www.elsevier.com/locate/physa An analysis of price impact function in orderdriven markets G. Iori a;, M.G. Daniels b, J.D. Farmer
More informationA8 Thermal properties of materials
A8 Thermal properties of materials Thermal properties the melting temperature, T m, and the glass temperature (temperatura de transição vítrea), T g, relate directly to the strength of the bonds in the
More informationMOBILE ROBOT TRACKING OF PREPLANNED PATHS. Department of Computer Science, York University, Heslington, York, Y010 5DD, UK (email:nep@cs.york.ac.
MOBILE ROBOT TRACKING OF PREPLANNED PATHS N. E. Pears Department of Computer Science, York University, Heslington, York, Y010 5DD, UK (email:nep@cs.york.ac.uk) 1 Abstract A method of mobile robot steering
More informationHow is a vector rotated?
How is a vector rotated? V. Balakrishnan Department of Physics, Indian Institute of Technology, Madras 600 036 Appeared in Resonance, Vol. 4, No. 10, pp. 6168 (1999) Introduction In an earlier series
More informationNMR and IR spectra & vibrational analysis
Lab 5: NMR and IR spectra & vibrational analysis A brief theoretical background 1 Some of the available chemical quantum methods for calculating NMR chemical shifts are based on the HartreeFock selfconsistent
More informationCFD SIMULATION OF SDHW STORAGE TANK WITH AND WITHOUT HEATER
International Journal of Advancements in Research & Technology, Volume 1, Issue2, July2012 1 CFD SIMULATION OF SDHW STORAGE TANK WITH AND WITHOUT HEATER ABSTRACT (1) Mr. Mainak Bhaumik M.E. (Thermal Engg.)
More informationVARIANCE REDUCTION TECHNIQUES FOR IMPLICIT MONTE CARLO SIMULATIONS
VARIANCE REDUCTION TECHNIQUES FOR IMPLICIT MONTE CARLO SIMULATIONS An Undergraduate Research Scholars Thesis by JACOB TAYLOR LANDMAN Submitted to Honors and Undergraduate Research Texas A&M University
More informationHigh School Algebra 1 Common Core Standards & Learning Targets
High School Algebra 1 Common Core Standards & Learning Targets Unit 1: Relationships between Quantities and Reasoning with Equations CCS Standards: Quantities NQ.1. Use units as a way to understand problems
More informationIn order to solve this problem it is first necessary to use Equation 5.5: x 2 Dt. = 1 erf. = 1.30, and x = 2 mm = 2 103 m. Thus,
5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,
More informationDiagrams and Graphs of Statistical Data
Diagrams and Graphs of Statistical Data One of the most effective and interesting alternative way in which a statistical data may be presented is through diagrams and graphs. There are several ways in
More informationEVALUATION METHODS OF DILATOMETER CURVES OF PHASE TRANSFORMATIONS
EVALUATION METHODS OF DILATOMETER CURVES OF PHASE TRANSFORMATIONS Petr MOTYČKA 1, Michal KÖVÉR 1,2 1 COMTES FHT a.s., Průmyslová 995, Dobřany, Czech Republic, 2 Slovak University of Technology in Bratislava,
More informationHow to Graph Trigonometric Functions
How to Graph Trigonometric Functions This handout includes instructions for graphing processes of basic, amplitude shifts, horizontal shifts, and vertical shifts of trigonometric functions. The Unit Circle
More informationHow to Win the Stock Market Game
How to Win the Stock Market Game 1 Developing ShortTerm Stock Trading Strategies by Vladimir Daragan PART 1 Table of Contents 1. Introduction 2. Comparison of trading strategies 3. Return per trade 4.
More information